LMucko/crystallography-open-database huggingface dataset:
Synthesis, spectroscopic, thermal and structural characterization of complex ferrocyanides K Ln Fe(II) (C N)6 * 3.5(H2 O) (Ln = Gd - Ho)
Goubard, F.; Tabuteau, A.; Structural Chemistry 14 (2003) 257–262; doi:

data_1533433
_publ_section_title
;
 Synthesis, spectroscopic, thermal and structural characterization of
 complex ferrocyanides K Ln Fe(II) (C N)6 * 3.5(H2 O) (Ln = Gd - Ho)
;
_journal_name_full               'Structural Chemistry'
_journal_page_first              257
_journal_page_last               262
_journal_volume                  14
_journal_year                    2003
_chemical_formula_sum            'C6 H6.96 Fe K N6 O3.48 Tb'
_chemical_name_systematic        'K Tb (Fe (C N)6) (H2 O)3.48'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.2714
_cell_length_b                   12.5153
_cell_length_c                   13.5954
_cell_volume                     1237.232
_citation_journal_id_ASTM        STCHES
_cod_data_source_file            Goubard_STCHES_2003_1037.cif
_cod_data_source_block           C6H6.96Fe1K1N6O3.48Tb1
_cod_original_formula_sum        'C6 H6.96 Fe1 K1 N6 O3.48 Tb1'
_cod_database_code               1533433
Preparation and structural study from neutron diffraction data of R2 Mo O6 ( R= Dy, Ho, Er, Tm, Yb, Y )
Alonso, J.A.; Pomjakushin, V.; Martinez-Lope, M.J.; Rivillas, F.; Journal of Solid State Chemistry 177 (2004) 2470–2476; doi:

data_1533434
_publ_section_title
;
 Preparation and structural study from neutron diffraction data of R2 Mo
 O6 ( R= Dy, Ho, Er, Tm, Yb, Y )
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              2470
_journal_page_last               2476
_journal_volume                  177
_journal_year                    2004
_chemical_formula_sum            'Er2 Mo O6'
_chemical_name_systematic        'Er2 (Mo O6)'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 108.617
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   16.3249
_cell_length_b                   10.9856
_cell_length_c                   5.3307
_cell_volume                     905.977
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Alonso_JSSCBI_2004_1779.cif
_cod_data_source_block           Er2Mo1O6
_cod_original_cell_volume        905.9775
_cod_original_formula_sum        'Er2 Mo1 O6'
_cod_database_code               1533434
Thermal decomposition of the methoxide complexes Mo O (O Me)4, Re4 O6 (O Me)12 and (Re1-x Mox) O6 (O Me)12 (0.24 < x < 0.55)
Seisenbaeva, G.A.; Sundberg, M.; Nygren, M.; Dubrovinsky, L.; Kessler, V.G.; Materials Chemistry and Physics 87 (2004) 142–148; doi:

data_1533435
_publ_section_title
;
 Thermal decomposition of the methoxide complexes Mo O (O Me)4, Re4 O6 (O
 Me)12 and (Re1-x Mox) O6 (O Me)12 (0.24 < x < 0.55)
;
_journal_name_full               'Materials Chemistry and Physics'
_journal_page_first              142
_journal_page_last               148
_journal_volume                  87
_journal_year                    2004
_chemical_formula_sum            'Mo O2'
_space_group_IT_number           136
_symmetry_space_group_name_Hall  '-P 4n 2n'
_symmetry_space_group_name_H-M   'P 42/m n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.8473
_cell_length_b                   4.8473
_cell_length_c                   2.8136
_cell_volume                     66.109
_citation_journal_id_ASTM        MCHPDR
_cod_data_source_file            Seisenbaeva_MCHPDR_2004_1898.cif
_cod_data_source_block           Mo1O2
_cod_original_cell_volume        66.10924
_cod_original_formula_sum        'Mo1 O2'
_cod_database_code               1533435
Synthesis, spectroscopic, thermal and structural characterization of complex ferrocyanides K Ln Fe(II) (C N)6 * 3.5(H2 O) (Ln = Gd - Ho)
Goubard, F.; Tabuteau, A.; Structural Chemistry 14 (2003) 257–262; doi:

data_1533436
_publ_section_title
;
 Synthesis, spectroscopic, thermal and structural characterization of
 complex ferrocyanides K Ln Fe(II) (C N)6 * 3.5(H2 O) (Ln = Gd - Ho)
;
_journal_name_full               'Structural Chemistry'
_journal_page_first              257
_journal_page_last               262
_journal_volume                  14
_journal_year                    2003
_chemical_formula_sum            'C6 H6.984 Dy Fe K N6 O3.492'
_chemical_name_systematic        'K Dy (Fe (C N)6) (H2 O)3.492'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.2583
_cell_length_b                   12.5089
_cell_length_c                   13.5474
_cell_volume                     1230.014
_citation_journal_id_ASTM        STCHES
_cod_data_source_file            Goubard_STCHES_2003_1038.cif
_cod_data_source_block           C6H6.984Dy1Fe1K1N6O3.492
_cod_original_formula_sum        'C6 H6.984 Dy1 Fe1 K1 N6 O3.492'
_cod_database_code               1533436
Preparation and structural study from neutron diffraction data of R2 Mo O6 ( R= Dy, Ho, Er, Tm, Yb, Y )
Alonso, J.A.; Rivillas, F.; Martinez-Lope, M.J.; Pomjakushin, V.; Journal of Solid State Chemistry 177 (2004) 2470–2476; doi:

data_1533437
_publ_section_title
;
 Preparation and structural study from neutron diffraction data of R2 Mo
 O6 ( R= Dy, Ho, Er, Tm, Yb, Y )
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              2470
_journal_page_last               2476
_journal_volume                  177
_journal_year                    2004
_chemical_formula_sum            'Mo O6 Tm2'
_chemical_name_systematic        'Tm2 (Mo O6)'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 108.654
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   16.2809
_cell_length_b                   10.9382
_cell_length_c                   5.312
_cell_volume                     896.286
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Alonso_JSSCBI_2004_1780.cif
_cod_data_source_block           Mo1O6Tm2
_cod_original_cell_volume        896.2859
_cod_original_formula_sum        'Mo1 O6 Tm2'
_cod_database_code               1533437
Crystal structure and charge order below the metal-insulator transition in the vanadium bronze beta-(Sr V6 O15)
Sellier, C.; Boucher, F.; Janod, E.; Solid State Sciences 5 (2003) 591–599; doi:

data_1533438
_publ_section_title
;
 Crystal structure and charge order below the metal-insulator transition
 in the vanadium bronze beta-(Sr V6 O15)
;
_journal_name_full               'Solid State Sciences'
_journal_page_first              591
_journal_page_last               599
_journal_volume                  5
_journal_year                    2003
_chemical_formula_sum            'O15 Sr V6'
_chemical_name_systematic        'Sr (V6 O15)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 109.42
_cell_angle_gamma                90
_cell_formula_units_Z            12
_cell_length_a                   15.411
_cell_length_b                   21.8809
_cell_length_c                   10.15
_cell_volume                     3227.921
_citation_journal_id_ASTM        SSSCFJ
_cod_data_source_file            Sellier_SSSCFJ_2003_1021.cif
_cod_data_source_block           O15Sr1V6
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_original_formula_sum        'O15 Sr1 V6'
_cod_database_code               1533438
Synthesis, spectroscopic, thermal and structural characterization of complex ferrocyanides K Ln Fe(II) (C N)6 * 3.5(H2 O) (Ln = Gd - Ho)
Goubard, F.; Tabuteau, A.; Structural Chemistry 14 (2003) 257–262; doi:

data_1533439
_publ_section_title
;
 Synthesis, spectroscopic, thermal and structural characterization of
 complex ferrocyanides K Ln Fe(II) (C N)6 * 3.5(H2 O) (Ln = Gd - Ho)
;
_journal_name_full               'Structural Chemistry'
_journal_page_first              257
_journal_page_last               262
_journal_volume                  14
_journal_year                    2003
_chemical_formula_sum            'C6 H7.08 Fe Ho K N6 O3.54'
_chemical_name_systematic        'K Ho (Fe (C N)6) (H2 O)3.54'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.2642
_cell_length_b                   12.5076
_cell_length_c                   13.5142
_cell_volume                     1227.869
_citation_journal_id_ASTM        STCHES
_cod_data_source_file            Goubard_STCHES_2003_1039.cif
_cod_data_source_block           C6H7.08Fe1Ho1K1N6O3.54
_cod_original_formula_sum        'C6 H7.08 Fe1 Ho1 K1 N6 O3.54'
_cod_database_code               1533439
Preparation and structural study from neutron diffraction data of R2 Mo O6 ( R= Dy, Ho, Er, Tm, Yb, Y )
Alonso, J.A.; Rivillas, F.; Pomjakushin, V.; Martinez-Lope, M.J.; Journal of Solid State Chemistry 177 (2004) 2470–2476; doi:

data_1533440
_publ_section_title
;
 Preparation and structural study from neutron diffraction data of R2 Mo
 O6 ( R= Dy, Ho, Er, Tm, Yb, Y )
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              2470
_journal_page_last               2476
_journal_volume                  177
_journal_year                    2004
_chemical_formula_sum            'Mo O6 Yb2'
_chemical_name_systematic        'Yb2 (Mo O6)'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 108.649
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   16.2437
_cell_length_b                   10.8992
_cell_length_c                   5.2907
_cell_volume                     887.503
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Alonso_JSSCBI_2004_1781.cif
_cod_data_source_block           Mo1O6Yb2
_cod_original_cell_volume        887.5029
_cod_original_formula_sum        'Mo1 O6 Yb2'
_cod_database_code               1533440
High-temperature crystal structure of wairakite
Seryotkin, Y.V.; Belitsky, I.A.; Joswig, W.; Bakakin, V.V.; Fursenko, B.A.; European Journal of Mineralogy (1,1989-) 15 (2003) 475–484; doi:

data_1533441
_publ_section_title
;
 High-temperature crystal structure of wairakite
;
_journal_name_full               'European Journal of Mineralogy (1,1989-)'
_journal_page_first              475
_journal_page_last               484
_journal_volume                  15
_journal_year                    2003
_chemical_formula_sum            'Al2 Ca0.959 H3.64 O13.82 Si4'
_chemical_name_systematic        'Ca0.959 (Al2 Si4 O12) (H2 O)1.82'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-I 2ya'
_symmetry_space_group_name_H-M   'I 1 2/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.5
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   13.666
_cell_length_b                   13.623
_cell_length_c                   13.531
_cell_volume                     2518.996
_citation_journal_id_ASTM        EJMIER
_cod_data_source_file            Seryotkin_EJMIER_2003_723.cif
_cod_data_source_block           H3.64Al2Ca0.959O13.82Si4
_cod_original_sg_symbol_Hall     '-C 2yc (x+z,y,-x)'
_cod_original_formula_sum        'H3.64 Al2 Ca0.959 O13.82 Si4'
_cod_database_code               1533441
Thermal expansion and thermally induced variations of the crystal structure of Al P O4 low crystobalite
Graetsch, H.A.; Neues Jahrbuch fuer Mineralogie. Monatshefte (Band=Jahr) (1950-) 2003 (2003) 289–301; doi:

data_1533442
_publ_section_title
;
 Thermal expansion and thermally induced variations of the crystal
 structure of Al P O4 low crystobalite
;
_journal_name_full
;
Neues Jahrbuch fuer Mineralogie. Monatshefte (Band=Jahr) (1950-)
;
_journal_page_first              289
_journal_page_last               301
_journal_volume                  2003
_journal_year                    2003
_chemical_formula_sum            'Al O4 P'
_chemical_name_systematic        'Al (P O4)'
_space_group_IT_number           20
_symmetry_space_group_name_Hall  'C 2c 2'
_symmetry_space_group_name_H-M   'C 2 2 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.1023
_cell_length_b                   7.0956
_cell_length_c                   7.0146
_cell_volume                     353.501
_citation_journal_id_ASTM        NJMMAW
_cod_data_source_file            Graetsch_NJMMAW_2003_864.cif
_cod_data_source_block           Al1O4P1
_cod_original_cell_volume        353.5013
_cod_original_formula_sum        'Al1 O4 P1'
_cod_database_code               1533442
Preparation and structural study from neutron diffraction data of R2 Mo O6 ( R= Dy, Ho, Er, Tm, Yb, Y )
Alonso, J.A.; Rivillas, F.; Martinez-Lope, M.J.; Pomjakushin, V.; Journal of Solid State Chemistry 177 (2004) 2470–2476; doi:

data_1533443
_publ_section_title
;
 Preparation and structural study from neutron diffraction data of R2 Mo
 O6 ( R= Dy, Ho, Er, Tm, Yb, Y )
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              2470
_journal_page_last               2476
_journal_volume                  177
_journal_year                    2004
_chemical_formula_sum            'Mo O6 Y2'
_chemical_name_systematic        'Y2 (Mo O6)'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 108.523
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   16.3538
_cell_length_b                   11.0183
_cell_length_c                   5.3506
_cell_volume                     914.185
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Alonso_JSSCBI_2004_1782.cif
_cod_data_source_block           Mo1O6Y2
_cod_original_cell_volume        914.1847
_cod_original_formula_sum        'Mo1 O6 Y2'
_cod_database_code               1533443
Synthesis, structure, electric transport and magnetic properties of Sr3 Mn Ti O7-d
Sharma, I.B.; Singh, C.; Singh, D.; Journal of Alloys Compd. 375 (2004) 11–14; doi:

data_1533444
_publ_section_title
;
 Synthesis, structure, electric transport and magnetic properties of Sr3
 Mn Ti O7-d
;
_journal_name_full               'Journal of Alloys Compd.'
_journal_page_first              11
_journal_page_last               14
_journal_volume                  375
_journal_year                    2004
_chemical_formula_sum            'Mn O6.891 Sr3 Ti'
_chemical_name_systematic        'Sr3 (Mn Ti O6.891)'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.8488
_cell_length_b                   3.8488
_cell_length_c                   20.1627
_cell_volume                     298.675
_citation_journal_id_ASTM        JALCEU
_cod_data_source_file            Sharma_JALCEU_2004_1517.cif
_cod_data_source_block           Mn1O6.891Sr3Ti1
_cod_original_cell_volume        298.6754
_cod_original_formula_sum        'Mn1 O6.891 Sr3 Ti1'
_cod_database_code               1533444
Formation, structure and hard magnetic properties of Sm2 Fe17-x Cox Cy compounds
Altounian, Z.; Liu Xubo; Girt, E.; Journal of Physics: Condensed Matter 15 (2003) 3315–3322; doi:

data_1533445
_publ_section_title
;
 Formation, structure and hard magnetic properties of Sm2 Fe17-x Cox Cy
 compounds
;
_journal_name_full               'Journal of Physics: Condensed Matter'
_journal_page_first              3315
_journal_page_last               3322
_journal_volume                  15
_journal_year                    2003
_chemical_formula_sum            'C0.75 Co5 Fe12 Sm2'
_chemical_name_systematic        'Sm2 Fe12 Co5 C0.75'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   8.5301
_cell_length_b                   8.5301
_cell_length_c                   12.4348
_cell_volume                     783.570
_citation_journal_id_ASTM        JCOMEL
_cod_data_source_file            Altounian_JCOMEL_2003_747.cif
_cod_data_source_block           C0.75Co5Fe12Sm2
_cod_original_cell_volume        783.5698
_cod_database_code               1533445
Crystal structure of three polymorphs of Y (P O3)3
Graia, M.; Driss, A.; Jouini, T.; Solid State Sciences 5 (2003) 393–402; doi:

data_1533446
_publ_section_title
;
 Crystal structure of three polymorphs of Y (P O3)3
;
_journal_name_full               'Solid State Sciences'
_journal_page_first              393
_journal_page_last               402
_journal_volume                  5
_journal_year                    2003
_chemical_formula_sum            'O9 P3 Y'
_chemical_name_systematic        'Y (P O3)3'
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            24
_cell_length_a                   21.042
_cell_length_b                   21.042
_cell_length_c                   12.159
_cell_volume                     4662.325
_citation_journal_id_ASTM        SSSCFJ
_cod_data_source_file            Graia_SSSCFJ_2003_1002.cif
_cod_data_source_block           O9P3Y1
_cod_original_formula_sum        'O9 P3 Y1'
_cod_database_code               1533446
Crystal structure of novel ferromagnetic La Fe13-x Gax C compounds
Shcherbakova, Ye.V.; Ivanova, G.V.; Gaviko, V.S.; Gabay, A.M.; Journal of Magnetism and Magnetic Materials 267 (2003) 26–34; doi:

data_1533447
_publ_section_title
;
 Crystal structure of novel ferromagnetic La Fe13-x Gax C compounds
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              26
_journal_page_last               34
_journal_volume                  267
_journal_year                    2003
_chemical_formula_sum            'C0.93 Fe10.04 Ga2.96 La'
_chemical_name_systematic        'La Fe10.04 Ga2.96 C0.93'
_space_group_IT_number           226
_symmetry_space_group_name_Hall  '-F 4a 2 3'
_symmetry_space_group_name_H-M   'F m -3 c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.805
_cell_length_b                   11.805
_cell_length_c                   11.805
_cell_volume                     1645.121
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            Shcherbakova_JMMMDC_2003_1592.cif
_cod_data_source_block           C0.93Fe10.04Ga2.96La1
_cod_original_cell_volume        1645.122
_cod_original_formula_sum        'C0.93 Fe10.04 Ga2.96 La1'
_cod_database_code               1533447
Structural investigation of trimethylammonium tetrachloromercurate
Amami, M.; Sebald, A.; van Smaalen, S.; Ben Salah, A.; Helluy, X.; Journal of Solid State Chemistry 177 (2004) 2961–2970; doi:

data_1533448
_publ_section_title
;
 Structural investigation of trimethylammonium tetrachloromercurate
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              2961
_journal_page_last               2970
_journal_volume                  177
_journal_year                    2004
_chemical_formula_sum            'C6 H20 Cl4 Hg N2'
_chemical_name_systematic        '(N H (C H3)3)2 (Hg Cl4)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2n'
_symmetry_space_group_name_H-M   'P 1 1 21/n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                92.2
_cell_formula_units_Z            4
_cell_length_a                   18.36
_cell_length_b                   6.164
_cell_length_c                   13.07
_cell_volume                     1478.055
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Amami_JSSCBI_2004_1849.cif
_cod_data_source_block           C6H20Cl4Hg1N2
_cod_original_sg_symbol_Hall     '-P 2ybc (z,x-z,y)'
_cod_original_formula_sum        'C6 H20 Cl4 Hg1 N2'
_cod_database_code               1533448
Crystal structure of three polymorphs of Y (P O3)3
Graia, M.; Driss, A.; Jouini, T.; Solid State Sciences 5 (2003) 393–402; doi:

data_1533449
_publ_section_title
;
 Crystal structure of three polymorphs of Y (P O3)3
;
_journal_name_full               'Solid State Sciences'
_journal_page_first              393
_journal_page_last               402
_journal_volume                  5
_journal_year                    2003
_chemical_formula_sum            'O9 P3 Y'
_chemical_name_systematic        'Y (P O3)3'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 127.597
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.176
_cell_length_b                   6.7075
_cell_length_c                   10.0853
_cell_volume                     759.809
_citation_journal_id_ASTM        SSSCFJ
_cod_data_source_file            Graia_SSSCFJ_2003_1003.cif
_cod_data_source_block           O9P3Y1
_cod_original_cell_volume        759.8094
_cod_original_formula_sum        'O9 P3 Y1'
_cod_database_code               1533449
Crystal structure of novel ferromagnetic La Fe13-x Gax C compounds
Shcherbakova, Ye.V.; Ivanova, G.V.; Gaviko, V.S.; Gabay, A.M.; Journal of Magnetism and Magnetic Materials 267 (2003) 26–34; doi:

data_1533450
_publ_section_title
;
 Crystal structure of novel ferromagnetic La Fe13-x Gax C compounds
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              26
_journal_page_last               34
_journal_volume                  267
_journal_year                    2003
_chemical_formula_sum            'C1.02 Fe10.052 Ga2.948 La'
_chemical_name_systematic        'La Fe10.052 Ga2.948 C1.02'
_space_group_IT_number           140
_symmetry_space_group_name_Hall  '-I 4 2c'
_symmetry_space_group_name_H-M   'I 4/m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.405
_cell_length_b                   8.405
_cell_length_c                   11.7
_cell_volume                     826.535
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            Shcherbakova_JMMMDC_2003_1593.cif
_cod_data_source_block           C1.02Fe10.052Ga2.948La1
_cod_original_formula_sum        'C1.02 Fe10.052 Ga2.948 La1'
_cod_database_code               1533450